Carbohydrate Polymers 115 (2015) 457–464
Contents lists available at ScienceDirect
Carbohydrate Polymers journal homepage: www.elsevier.com/locate/carbpol
Preparation and characterization of functionalized cellulose nanocrystals Assya Boujemaoui, Surinthra Mongkhontreerat, Eva Malmström ∗ , Anna Carlmark ∗ KTH Royal Institute of Technology, School of Chemical Science and Engineering, Fibre and Polymer Technology, Teknikringen 56, SE-100 44 Stockholm, Sweden
a r t i c l e
i n f o
Article history: Received 13 June 2014 Received in revised form 22 August 2014 Accepted 25 August 2014 Available online 18 September 2014 Keywords: Acid hydrolysis Cellulose nanocrystals Esteriﬁcation Functionalization Functional organic acid
a b s t r a c t In this work, a series of functional nanocrystals (F-CNCs) was successfully produced by an efﬁcient preparation method, combining acid hydrolysis and Fischer esteriﬁcation with various organic acids. Functionalities such as ATRP initiators, double bonds, triple bonds, and thiols could be incorporated on CNCs. Surface modiﬁcation was conﬁrmed by FT-IR, XPS, and elemental analysis. Physical properties of FCNCs were assessed by AFM, XRD and TGA. Moreover, ATRP initiator functionalized CNCs were utilized to graft poly(methyl methacrylate) via ATRP, thiol functionalized CNCs were reacted with Ellman’s reagent to determine the thiol content and dye disperse red 13 was attached to alkyne functionalized CNCs to estimate the propiolate content. The herein presented method is a highly versatile and straightforward procedure for the preparation of F-CNCs which is believed to be a better alternative for the commonly utilized, extensive, multistep, and time consuming post functionalization methods. © 2014 Elsevier Ltd. All rights reserved.
1. Introduction During the last decade, cellulose nanocrystals (CNCs) have attracted great interest, in both industry and academia, owing to their low density, renewability, biodegradability, high reinforcing capability, lower production cost compared to glass and carbon nanoﬁbers, and their vast applicability (Mariano, El Kissi, & Dufresne, 2014). CNCs were originally prepared by acid hydrolysis employing strong acids, mainly sulfuric and hydrochloric acids (Rånby, 1951). The acid hydrolysis conditions has thereafter been optimized in order to improve the recovery yield and to tailor the CNCs dimensions (Bondeson, Mathew, & Oksman, 2006). Recently, phosphoric acid was utilized to prepare CNCs (Camarero Espinosa, Kuhnt, Foster, & Weder, 2013). Several other preparation methods have been reported, such as combination of acid and enzymatic hydrolysis (Siqueira, Tapin-Lingua, Bras, da Silva Perez, & Dufresne, 2010), TEMPO oxidation (Hirota, Tamura, Saito, & Isogai, 2010; Qin, Tong, Chin, & Zhou, 2011), ammonium persulfate oxidation (Leung et al., 2011), ionic liquid hydrolysis (Man et al., 2011), and gaseous acid hydrolysis (Nuopponen, Meriluoto, & Kontturi, 2012). However, acid hydrolysis is the most widely used procedure for the production of CNCs. CNCs exhibit a high speciﬁc surface area
∗ Corresponding authors. Tel.: +46 8 7908027 (AC), +46 8 7907225 (EM). E-mail addresses: [email protected]
(E. Malmström), [email protected]
(A. Carlmark). http://dx.doi.org/10.1016/j.carbpol.2014.08.110 0144-8617/© 2014 Elsevier Ltd. All rights reserved.
that implicates more available hydroxyl groups on their surface and subsequently offers great possibility for chemical modiﬁcation (Dufresne, 2012). The application potential of CNCs can be signiﬁcantly enhanced by surface modiﬁcation (Eichhorn, 2011). A series of surface modiﬁed CNCs with outstanding properties has previously been prepared either by covalent or non-covalent chemical modiﬁcation approaches (Habibi, 2014). The non-covalent approach is based on the adsorption of surfactants to the cellulose surface and can be accomplished via ionic or non-ionic interactions. This method is used mainly to improve the dispersibility of CNCs in organic solvents and hydrophobic matrices (Aloulou, Bouﬁ, & Beneventi, 2004; Ben Azouz, Ramires, Van den Fonteyne, El Kissi, & Dufresne, 2011; Cranston & Gray, 2006; Habibi, Hoeger, Kelley, & Rojas, 2009; Kim et al., 2009; Salajková, Berglund, & Zhou, 2012). For the covalent modiﬁcation, small molecules or polymers are reacted with the hydroxyl groups on the glucose units. For example, CNC surfaces have been modiﬁed by grafting of polyesters (poly(-caprolactone and polylactide) via ring-opening polymerization of cyclic esters utilizing the OH-group as an initiating function (Carlmark, Larsson, & Malmström, 2012). Moreover, different functional groups have been attached to CNC surfaces, such as initiators for reversible deactivation radical polymerization (RDRP), (Morandi, Heath, & Thielemans, 2009; Yi, Xu, Zhang, & Zhang, 2009; Zoppe et al., 2010) allyl, thiol, alkyne, and azide functionalities for click chemistry reactions (Filpponen & Argyropoulos, 2010; Huang, Li, & Gray, 2014; Sadeghifar, Filpponen, Clarke, Brougham,
A. Boujemaoui et al. / Carbohydrate Polymers 115 (2015) 457–464
& Argyropoulos, 2011; Tingaut, Hauert, & Zimmermann, 2011) via esteriﬁcation reaction of available hydroxyl groups of cellulose with acid halides. Amine groups were also grafted on CNCs surface via esteriﬁcation reaction followed by thiol-ene Michael addition (Nielsen, Eyley, Thielemans, & Aylott, 2010). Furthermore, functionalized CNCs can be employed for polymer grafting via RDRP, to enhance the compatibility of CNCs and a hosting matrix, ﬂuorescent labeling of CNCs for bioimaging applications, cellulosic photo responsive nano-arrays (Filpponen, Sadeghifar, & Argyropoulos, 2011), as well as several other applications (Biyani, Foster, & Weder, 2013; Kelly et al., 2013; Khan et al., 2013; Shopsowitz, Hamad, & MacLachlan, 2011). However, the above mentioned functionalities have all been prepared by the reaction of already produced CNCs. To introduce functionalities on already prepared CNCs, multiple steps and tedious liquid exchange from water to an appropriate reaction solvent, puriﬁcation and then re-dispersion are commonly required. In this procedure, typically, unmodiﬁed CNCs are prepared by acid hydrolysis of cellulose ﬁbers in an initial step, followed by solvent exchange into organic solvents or freeze drying and re-dispersion, and then, in a second step, the CNCs are post-functionalized to attach the functional group. In a previous study by Dorgan et al., simultaneous Fisher esteriﬁcation and acid hydrolysis were performed in order to produce functional cellulose nanocrystals (F-CNCs) but this approach was only applied for introducing acetate and butyrate groups (Braun & Dorgan, 2008). The aim of this study was to prepare a series of F-CNCs where the functionality is introduced onto the CNCs already in the production step, by utilizing functional organic acids. In this simple and versatile manner, modiﬁed CNCs bearing functional groups such as; double and triple bonds, thiols and a bromo-ester group (i.e. initiator for atom transfer radical polymerization, ATRP) were produced in relatively high yields (46–62 wt%) (Braun & Dorgan, 2008). We hypothesize that the surface functionalization of CNCs involves Fischer esteriﬁcation and hydrolysis reactions. Consequently F-CNCs could be directly obtained in a one-step reaction, thus omitting extra functionalization steps and tedious solvent exchange. The properties and reactivity of F-CNCs were also investigated. We believe this study to be of utmost importance for the chemical modiﬁcation of CNCs and hence for the production of functional CNCs. The incorporated functionalities allow for CNCs to be utilized in composite applications, either compatibilizing the surface of the ﬁbers with the matrix material, or by introducing cross-linkable groups. Furthermore, the CNCs functionalized with an ATRP-initiator could be polymerized with a plethora of functional polymers, resulting in new and interesting materials.
2. Experimental and methods
2.2. Instrumentation Size exclusion chromatography (SEC) with dimethyl formamide (DMF) as mobile phase was utilized to determine molecular weights and molar-mass dispersities. The analyses were performed on a TOSOH EcoSEC HLC-8320 GPC system equipped with an EcoSEC ˚ RI detector and three columns (PSS PFG 5 m; Microguard, 100 A, ˚ (MW resolving range: 100–300,000 g mol−1 ) from PSS and 300 A) GmbH, using DMF (0.2 mL min−1 ) with 0.01 M LiBr as the mobile phase at 50 ◦ C. A conventional calibration method was created using narrow, linear poly(methyl methacrylate) standards ranging from 700 to 2000,000 g mol−1 . Corrections for ﬂow rate ﬂuctuations were made using toluene as an internal standard. PSS WinGPC Unity software version 7.2 was used to process data. IR spectroscopy was performed on a Perkin-Elmer Spectrum 2000 FT-IR equipped with a MKII Golden Gate, Single Reﬂection ATR system from Specac Ltd, London, U.K. All spectra were normalized against a speciﬁc ATR crystal absorption region (2300–1900 cm−1 ). Proton Nuclear Magnetic Resonance (1 H NMR) was conducted on a Bruker AM 400 at 400 MHz using deuturated chloroform (CDCl3 ) as solvent to determine the conversion of the non-grafted PMMA. The solvent signal was used as an internal standard. The molecular weight (Mn,th ) of PMMA chains was estimated from the degree of polymerization (DP) assessed by 1 H NMR. Atomic force microscopy (AFM) with tapping-mode AFM (Multimode IIIa, Veeco Instruments, Santa Barbara, CA) was utilized to determine the CNCs dimensions. Diluted CNCs water dispersions were applied on modiﬁed surface mica with poly l-lysine 1% and the excess was washed with Milli-Q water. The sample surfaces were dried with air ﬂow and scanned with a cantilever having a tip radius